SUPERSEDED (click for Active standard)
| ||Format||Pages||Price|| |
|3||$45.60||  ADD TO CART|
1.1 This test method covers the testing of thin copper alloy strip to determine its formability or its ability to resist cracking when forming around a specific radius. The criterion for failure is the occurrence of cracks found on the outer radius of curvature (convex).
1.2 This bend test is limited to strip 0.003 to 0.031 in. thick. (0.076 to 0.79 mm)
1.3 The size of the forming radii used in this test shall be 0.005 to 0.250 in. (0.127 to 6.35 mm).
1.4 The values stated in inch-pounds are to be regarded as the standard. The values given in parentheses are for information only.
1.5 This standard does not purport to address all of the safety problems, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
B846 Terminology for Copper and Copper Alloys
B950 Guide for Editorial Procedures and Form of Product Specifications for Copper and Copper Alloys
E6 Terminology Relating to Methods of Mechanical Testing
E290 Test Methods for Bend Testing of Material for Ductility
ICS Number Code 77.150.30 (Copper products)
UNSPSC Code 30262400(Copper ingots strip billets and coil)
ASTM B820-98, Standard Test Method for Bend Test for Formability of Copper Alloy Spring Material, ASTM International, West Conshohocken, PA, 1998, www.astm.orgBack to Top